Post on 12-Oct-2015
Embed Size (px)
DESCRIPTIONREGENERATED FIBRES -: A fiber manufactured by dissolving a natural material, such as cellulose, and then restoring or regenerating the material through extrusion and precipitation. Cellulose, for example, is commonly regenerated to form rayon.VISCOSE RAYON Polymer Chemistry : The raw material for the production of Viscose rayon is wood pulp. However, the manufacturing process emits toxic effluents which have adverse environmental effects. Because of its cellulosic base , it has some properties which are similar to those of cotton and any other natural cellulosic fibres. It has moderate resistance to acids and alkalis. However, it may be damaged by relatively weak acids. Moreover, due to the inelasticity of fibers, it has poor abrasion resistance.
REGENERATED FIBRES -:A fiber manufactured by dissolving a natural material, such as cellulose, and then restoring or regenerating the material through extrusion and precipitation. Cellulose, for example, is commonly regenerated to form rayon.VISCOSE RAYON Polymer Chemistry : The raw material for the production of Viscose rayon is wood pulp. However, the manufacturing process emits toxic effluents which have adverse environmental effects. Because of its cellulosic base , it has some properties which are similar to those of cotton and any other natural cellulosic fibres. It has moderate resistance to acids and alkalis. However, it may be damaged by relatively weak acids. Moreover, due to the inelasticity of fibers, it has poor abrasion resistance. Technology (Figure 40.2): The raw materials used in this process are cellulose wood pulp sheets or cotton linters. These are placed in a steeping press with contact in aqueous NaOH Solution for a period of 2 4 hours at normal room temperature. A hydraulic ram presses out the excess alkali and the sheets are shredded to crumbs and aged for 2 3 days. The aging process has its direct consequence on the viscosity of the solution. Later CS2 is added in a rotating drum mixer over a period of 3 hours. The orange cellulose xanthate which forms is transferred to a solubilizer , wherein it is mixed into dilute caustic . The mixing of cellulose xanthate and dilute caustic yields a orange colored viscous solution which contains 7 8 % cellulose and 6.5 7 % NaOH. It is digested at room temperature for 4-5 days. Thereafter , the solution is filtered and fed to spinning machines. The spinning is carried out in extrusion spinnerettes , which are made up of platinum or gold alloys. The orifices of these spinnerets have a diameter of 0.1 0.2 mm. for continuous filament yarns and of diameter 0.05 0.1 mm for short fibre shapes. The solution extruded from the spinnerette is contacted with an acid bath which precipitates the filaments without causing them to break or stick together. The processing treatments of washing, desulphurizing, bleaching and conditioning takes place continuously and in order after the filaments are wound on a series of plastic rolls.
Figure 40.2 Manufacture of Viscose Rayon
Cellulose fibers are fibers from some plant or plant-based materials. They are usually categorized as "natural" or "manufactured".NaturalNatural cellulose fibers are fibers that are still recognizable as being from a part of the original plant because they are only processed as much as needed to clean the fibers for use. For example, cotton fibers look like the soft fluffy cotton balls that they come from. Linen fibers look like the strong fiberous strands of the flax plant. All "natural" fibers go through a process where they are separated from the parts of the plant that are not used for the end product, usually through harvesting, separating from chaff, scouring, etc.The presence of linear chains of thousands of glucose units linked together allows a great deal of hydrogen bonding between OH groups on adjacent chains, causing them to pack closely into cellulose fibers. As a result, cellulose exhibits little interaction with water or any other solvent. Cotton and wood, for example, are completely insoluble in water and have considerable mechanical strength. Since cellulose does not have a helical structure like amylose, it does not bind to iodine to form a colored product. They are usually categorized into two categoriesManufacturedManufactured cellulose fibers come from plants that are processed into a pulp and then extruded in the same ways that synthetic fibers like polyester or nylon are made. Rayon or viscose is one of the most common "manufactured" cellulose fibers, and it can be made from wood pulp.TextileIn the textile industry regenerated cellulose is used as fibers such as rayon, (including modal, and the more recently developed Lyocell). Cellulose fibers are manufactured from dissolving pulp. Cellulose-based fibers are of two types, regenerated or pure cellulose such as from the cupro-ammonium process and modified cellulose such as the cellulose acetates.The first artificial fiber, known as artificial silk, became known as viscose around 1894, and finally rayon in 1924. A similar product known as cellulose acetate was discovered in 1865. Rayon and acetate are both artificial fibers, but not truly synthetic, being made from wood. Although these artificial fibers were discovered in the mid-nineteenth century, successful modern manufacture began much later.Environmental issues What is often marketed as "bamboo fiber" is actually not the fibers that grow in their natural form from the bamboo plants, but instead a highly processed bamboo pulp that is extruded as fibers. Although the process is not as environmentally friendly as "bamboo fiber" appears, planting & harvesting bamboo for fiber is much more sustainable and environmentally friendly than harvesting more slow growing trees and clearing existing forest habitats for timber plantations.
RAYON FIBERSUpdated: April, 2004 - Raghavendra R. Hegde, Atul Dahiya, M. G. Kamath(Praveen Kumar Jangala, Haoming Rong)1. INTRODUCTION Rayon is the oldest commercial manmade fiber. The U. S. Trade Commission defines rayon as "manmade textile fibers and filaments composed of regenerated cellulose". The process of making viscose was discovered by C.F.Cross and E.J.Bevan in 1891. The process used to make viscose can either be a continuous or batch process. The batch process is flexible in producing a wide variety of rayons, with broad versatility. Rayon's versatility is the result of the fiber being chemically and structurally engineered by making use of the properties of cellulose from which it is made. However, it is somewhat difficult to control uniformity between batches and it also requires high labor involvement. The continuous process is the main method for producing rayon. Three methods of production lead to distinctly different rayon fibers: viscose rayon, cuprammonium rayon and saponified cellulose acetate. Of the methods mentioned, the viscose method is relatively inexpensive and of particular significance in the production of nonwoven fabrics. According to the latest data from the fiber Economics Bureau, domestic producers shipments of rayon staple to nonwoven roll goods are shown in table 1.Table 1: Shipments of Rayon Staple to Nonwoven roll goods YearsMillions of pounds
2. VISCOSE RAYON The process of manufacturing viscose rayon consists of the following steps mentioned, in the order that they are carried out: (1) Steeping, (2) Pressing, (3) Shredding, (4) Aging, (5) Xanthation, (6) Dissolving, (7)Ripening, (8) Filtering, (9) Degassing, (10) Spinning, (11) Drawing, (12) Washing, (13) Cutting. The various steps involved in the process of manufacturing viscose are shown in Fig. 1, and clarified below.
Figure 1: Process of manufacture of viscose rayon fiberSteeping: Cellulose pulp is immersed in 17-20% aqueous sodium hydroxide (NaOH) at a temperature in the range of 18 to 25C in order to swell the cellulose fibers and to convert cellulose to alkali cellulose. (C6H10O5)n + nNaOH ---> (C6H9O4ONa)n + nH2O(2) Pressing: The swollen alkali cellulose mass is pressed to a wet weight equivalent of 2.5 to 3.0 times the original pulp weight to obtain an accurate ratio of alkali to cellulose.(3) Shredding: The pressed alkali cellulose is shredded mechanically to yield finely divided, fluffy particles called "crumbs". This step provides increased surface area of the alkali cellulose, thereby increasing its ability to react in the steps that follow.(4) Aging: The alkali cellulose is aged under controlled conditions of time and temperature (between 18 and 30 C) in order to depolymerize the cellulose to the desired degree of polymerization. In this step the average molecular weight of the original pulp is reduced by a factor of two to three. Reduction of the cellulose is done to get a viscose solution of right viscosity and cellulose concentration.(5) Xanthation: In this step the aged alkali cellulose crumbs are placed in vats and are allowed to react with carbon disulphide under controlled temperature (20 to 30C) to form cellulose xanthate.(C6H9O4ONa)n + nCS2 ----> (C6H9O4O-SC-SNa)n Side reactions that occur along with the conversion of alkali cellulose to cellulose xanthate are responsible for the orange color of the xanthate crumb and also the resulting viscose solution. The orange cellulose xanthate crumb is dissolved in dilute sodium hydroxide at 15 to 20 C under high-shear mixing conditions to obtain a viscous orange colored solution called "viscose", which is the basis for the manufacturing process. The viscose solution is then filtered (to get out the insoluble fiber material) and is deaerated. (6) Dissolving: The yellow crumb is dissolved in aqueous caustic solution. The large xanthate substituents on the cellulose force the chains apart, reducing the interchain hydrogen bonds and allowing water molecules to solvate and separate the chains, leading to solution of the otherwise insoluble cellulose. Because of the blocks of un-xanthated cellulose in the crystalline regions, the yellow crumb is not completely soluble at this stage. Because the cellulose xanthate solution (or more accurately, suspension) has a very high viscosity, it has been termed "viscose".(7) Ripening: The viscose is allowed to stand for a period of time to "ripen". Two important process occur during ripening: Redistribution and loss of xanthate groups. The reversible xanthation reaction allows some of the xanthate groups to revert to cellulosic hydroxyls and free CS2. This free CS2 can then escape or react with other hydroxyl on other portions of the cellulose cha